Journal of Hazardous Materials 167 (2009) 482–488 Contents lists available at ScienceDirect Journal of Hazardous Materials journal homepage: www.elsevier.com/locate/jhazmat Kinetics and equilibrium studies for the removal of nickel and zinc from aqueous solutions by ion exchange resins Bilge Alyüz ∗ , Sevil Veli University of Kocaeli, Department of Environmental Engineering, Kocaeli 41380, Turkey a r t i c l e i n f o Article history: Received 18 August 2008 Received in revised form 26 December 2008 Accepted 6 January 2009 Available online 15 January 2009 Keywords: Ion exchange Heavy metals Isotherms Kinetics Separation factors a b s t r a c t Removal of heavy metals from wastewater is obligatory in order to avoid water pollution. In the present study, performance of Dowex HCR S/S cation exchange resin was evaluated for removal of nickel and zinc from aqueous solutions. Batch shaking adsorption experiments were performed in order to examine the effects of pH, dosage of resin and contact time on removal process. It was observed that more than 98% removal efﬁciency was achieved under optimal conditions for nickel and zinc. The experimental equilibrium data were tested for the Langmuir, Freundlich and Temkin isotherms. Correlation coefﬁcients indicate the following order to ﬁt isotherms: Langmuir > Freundlich > Temkin for both nickel and zinc ions. Pseudo-ﬁrst- and -second-order kinetic models were used for describing kinetic data. It was determined that removal of Ni2+ and Zn2+ was wellﬁtted by second-order reaction kinetic. Furthermore, separation factors and distribution coefﬁcients of nickel and zinc for Dowex HCR S/S were calculated. © 2009 Elsevier B.V. All rights reserved. 1. Introduction The release of large quantities of heavy metals into the natural environment has resulted in a number of environmental problems. Toxic metals can be distinguished from other pollutants, since they are not biodegradable and can be accumulated in nature. They also cause various diseases and disorders when exceed speciﬁc limits [1,2]. Zinc is one of the most important pollutants for surface and ground water. Because of its acute toxicity and non-biodegradability, zinc-containing liquid and solid wastes are considered as hazardous wastes [3,4]. The nickel ion, compared with other heavy metals, is a more recalcitrant pollutant . As it is widely used in many industrial processes, removal of nickel from wastewaters gains importance. Metal treatment industries containing nickel in discharged waters, frequently use nickel in its sulfate form . This affects the decision of treatment method used for removal of nickel from wastewaters. Classical techniques of heavy metal removal from solutions include the following processes: precipitation, electrolytic methods, ion exchange, evaporation and adsorption . Among these methods ion exchange receives considerable interest with high efﬁciency and low operational costs. The main advantages of ion exchange over chemical precipitation are recovery of metal value, ∗ Corresponding author. Tel.: +90 262 3033253; fax: +90 262 3033003. E-mail address: [email protected] (B. Alyüz). 0304-3894/$ – see front matter © 2009 Elsevier B.V. All rights reserved. doi:10.1016/j.jhazmat.2009.01.006 selectivity, less sludge volume produced and the meeting of strict discharge speciﬁcations . Among the materials used in ion exchange processes, synthetic resins are commonly preferred as they are effective and inexpensive . Cation exchange resins generally contain sulfonic acid groups. These groups can also be carboxylic, phosphonic or phosphinic. Certain general rules for cation exchange are: (i) the exchanger prefers ions of high charge, (ii) ions of small hydrated volume are preferred and (iii) ions, which interacts strongly with the functional groups of the exchangers are preferred [10,11]. In literature, there have been various investigations about removal of heavy metals by ion exchange resins. Halle et al. observed that macroporous carboxylic cation exchanger Wofatit CA-20 in the sodium form exhibites high removal efﬁcieny for treatment of Ni(II) ions from washings formed during the nickel plating . Cu(II) ions are effectively removed from sea and river water by Amberlyst A-27 and Diaion PA-318, strongly basic anion exchangers and batocuproinodisulphonate as a chelating agent . Also, Dowex HCR S/S and Dowex Marathon C resins provided adsorption capacities of 26.27 mg/g and 46.55 mg/g for copper removal . Macroporous strongly basic anion exchangerLewatit MP-500A is characterized by high selectivity for Cr(VI) ions . Dowex HCR S/S type resins are in sodium form and due to their high cation exchange capacities they reduce the residual concentration of heavy metals below the discharge limits. They are also widely available as they are commercially produced. Furthermore their regeneration properties supply economical beneﬁts. Due to B. Alyüz, S. Veli / Journal of Hazardous Materials 167 (2009) 482–488 Nomenclature A B C Ce Co Ct CM2+ CNa+ D m M Temkin isotherm constant constant related with adsorption heat total ion concentration in solution equilibrium concentration of solution initial heavy metal concentration metal concentration at time t concentration of metal ions in solution concentration Na+ ions in solution distribution coefﬁcient amount of the resin Ni2+ or Zn2+ ions exchanging with Na+ ions in the solution phase k equilibrium constant of Langmuir isotherm k1 rate constant of pseudo-ﬁrst-order adsorption kinetic rate constant of pseudo-second-order adsorption k2 kinetic Freundlich isotherm constant Kf KM2+ /Na+ preference factor of metal ions for ion exchange process n adsorption intensity R2 correlation coefﬁcients t time xNa+ equivalence ratio of Na+ ions in solution V solution volume monolayer capacity for Langmuir isotherm Vm yNa+ equivalence ratio of Na+ ions in resin qe amount of adsorbed heavy metal per unit resin mass qM2+ concentration of metal ions in resin concentration of Na+ ions in resin qNa+ q total ion exchange capacity qe,calculated calculated value for amount of adsorbed heavy metal per unit resin mass qe,experimental experimental value for amount of adsorbed heavy metal per unit resin mass amount of heavy metal adsorbed at time t qt ˛ separation factor for nickel and zinc removal mentioned properties, in this study Dowex HCR S/S resin has been preferred. Batch technique was used in order to determine the equilibrium data. After deﬁning optimum reaction conditions (pH, resin dosage, contact time), experimental results were applied to Langmuir, Freundlich and Temkin isotherms. First- and second-order reaction kinetics were calculated for determination of adsorption mechanisms. Distrubution coefﬁcients and separation factors of nickel and zinc were also found for Dowex HCR S/S. It is thought that results of this study can be useful for treatment processes of sectors containing heavy metal in their wastewaters. 2. Experimental 2.1. Materials Analytical grade reagents were used in experimental studies. Nitrate salts of test metals (Zn(NO3 )2 ·6H2 O and Ni(NO3 )2 ·6H2 O from Merck) were used for preparing certain concentrations of synthetic solutions. pH adjustments were carried out by using 0.1N HCl and 0.1N NaOH. Dowex HCR S/S cation exchange resin was preferred as dowextype ion exchangers are durable, insoluble and compatible. The structural polymeric backbone of the resin is styrene cross-linked 483 Table 1 Characteristics of tested Dowex HCR S/S. Type Matrix Functional group Physical form Shipping weight Total exchange capacity Particle size Particle density Whole beads Ionic form as shipped Strong acid cation Styrene-DVB, gel Sulfonic acid Uniform particle size spherical beads 800 g/L Minimum 1.9 eq/L 0.3–1.2 mm: 90% minimum, <0.3 mm: 1% maximum 1.30 g/mL 90% minimum Na+ with divinyl benzene functionalized with a sulfonic acid functional group as the ion exchange site . Pysical and chemical properties of Dowex HCR S/S are given in Table 1. 2.2. Apparatus HACH DR 2000 spectrophotometer was used for the determination of remaining metal concentrations in solutions. Used methods were 1-(2 Pyridylazo)-2-Naphthol (PAN) Method (Method no: 8150) and Zincon Method (Method no: 8009) for nickel and zinc analyses, respectively. Batch experiments were carried out in NUVE shaker. Testo pH-meter was used for pH measurements. 2.3. Equilibrium studies The batch ion exchange experiments were performed in a wide variety of conditions including different pH, various resin dosages and agitation periods. Effects of each factor were determined keeping other variables constant. In the experiments 100 ml of synthetic solutions containing 100 mg/L of Ni(II) and Zn(II) were added into ﬂasks with different amounts of resin varying between 0.05 and 0.7 g. pH adjustments were made by using 0.1N sodium hydroxide and 0.1N hydrochloric acid. Solutions were shaked at 200 rpm for a predetermined period. Temparature was kept constant at 23 ◦ C during batch tests. At the end of agitation time resins were ﬁltered and metal contents of solutions were analyzed by spectrophotometer. 2.4. Isotherm studies The adsorption capacity was calculated using following formula: qe = (Co − Ce )V m (1) where qe (mg/g) is the equilibrium adsorption capacity, Co and Ce (mg/L) are the initial and equilibrium concentration of metal ions in solution, V (L) is the volume, and m (g) is the amount of the resin. By using this formula qe values for different metal concentrations were calculated. Relationship of qe versus Ce is shown in Fig. 1. Adsorption isotherm studies were carried out in a series of 250 mL reaction bottles. 100 mL of metal solutions were adjusted to 100 mg/L concentration. Resin amounts were kept constant at 0.2 and 0.3 g for nickel and zinc solutions. After reaching equilibrium, solutions were separated and analyzed. 2.5. Kinetic studies Kinetic experiments were made by using 100 mL of nickel and zinc solutions of various concentrations (50, 100, 150 mg/L). Samples were taken at different time intervals (0–300 min) and remaining metal concentrations were analyzed. The rate constants were calculated using conventional rate expressions. Following for- 484 B. Alyüz, S. Veli / Journal of Hazardous Materials 167 (2009) 482–488 Fig. 1. Relationship between equilibrium concentration and adsorption capacity. Fig. 3. Effect of pH on precipitation of metal hydroxides (Initial metal concentration 100 mg/L, without resin dosage, agitation period 2 h). mula was used to determine adsorbed metal concentration qt : qt = (Co − Ct )V m (2) where qt (mg/g) is the adsorption capacity at time t, Co (mg/L) is the initial metal concentration, Ct (mg/L) is the concentration of metal ions in solution at time t, V (L) is the volume, and m (g) is the amount of the resin. 3. Results and discussion 3.1. Effect of pH Hydronium ion concentration is an important parameter affecting the ion-exchange process. This is partly because hydrogen ions themselves are strongly competing adsorbate and the solution pH inﬂuences the ionization of surface functional groups. In order to investigate the effect of pH on removal of nickel and zinc by Dowex HCR S/S 100 ml of 100 mg/L metal solutions were used. Experiments were performed in the pH range 2–9. Constant resin amount (0.2 g) was added to all reaction bottles and solutions were agitated for 2 h at 200 rpm speed. Effect of pH on removal efﬁciency is shown in Fig. 2. As seen from Fig. 2. optimal uptake of Ni2+ and Zn2+ occurred at pH 4 and 6, respectively. At high pH values, decrease in removal efﬁciency achieved by resins can be described with formation of Ni(OH)2 and Zn(OH)2 during reaction of Ni2+ and Zn2+ ions with OH− . In this state, hydrolysis accompanied by precipitation of metal hydroxides may occur . In order to examine the effects of pH on precipitation, experiments without resin dosage were carried out. As seen from Fig. 3, Fig. 2. Effect of pH on removal of nickel and zinc by Dowex HCR S/S cation exchange resin. (Initial metal concentration 100 mg/L, resin dosage 0.2 g/100 mL, agitation period 2 h). at high pH values metal ions precipitate due to formation of metal hydroxides. 3.2. Effect of resin dosage The resin amount is also one of the important parameters to obtain the quantitative uptake of metal ion. The dependence of metal sorption on resin input amount was studied by varying the amount of Dowex HCR S/S (0.05–0.7 g), while the other parameters such as pH (pH 6 and 4 for nickel and zinc, respectively), initial metal concentration (100 mg/L) and stirring speed (200 rpm) remained constant. It was apparent that the adsorption percentage of metal ions increased with higher resin dosages and the removal efﬁciency of 99% was achieved by using 0.2–0.3 g/100 mL resin dosage for nickel and zinc (Fig. 4). This result proved that increasing the amount of adsorbent provides higher removal due to formation of greater adsorption sites. 3.3. Effect of agitation time Predetermined optimal values of pH and resin dosage were used for analyzing effects of time on removal process. Fig. 5 shows the dependence of removal efﬁciency with agitation time. The removal increases with time and attains equilibrium in 90 min for nickel and in 120 min for zinc with initial concentrations of 100 mg/L. It is clear that complete removal of nickel ions requires less residence time compared to zinc. Fig. 4. Effect of resin dosage on removal of nickel and zinc by Dowex HCR S/S cation exchange resin. (Initial metal concentration 100 mg/L, pH 4 and 6, agitation period 2 h). B. Alyüz, S. Veli / Journal of Hazardous Materials 167 (2009) 482–488 Fig. 5. Effect of contact time on removal of nickel and zinc by Dowex HCR S/S cation exchange resin. (Initial metal concentration 100 mg/L, pH 4 and 6, resin dosage 0.2 and 0.3 g). 3.4. Distribution coefﬁcients and separation factors In order to calculate distribution coefﬁcients and separation factors, batch experiments were carried out at optimal conditions (pH 4 and 6; resin dosage 0.2 and 0.3 g, respectively for nickel and zinc) by using 100 mL of 150 mg/L metal solutions. Distribution coefﬁcients were determined by the formula given below : amount on resin mL of solution D= × amount in solution g of dry resin (3) Calculated distribution coefﬁcients were quite high for both nickel (5.80 × 104 ) and zinc (2.25 × 104 ) ions. Exchanging ions of unequal charge as in the case with the exchange of Na+ with the solution phase Ni2+ or Zn2+ (represented with M2+ ) can be expressed as: 2+ + + M2+ s + 2Nar → Mr + 2Nas (4) where subscripts s and r refer to “solution” and “resin” phases, respectively. In ion exchange processes, selectivity can be quantiﬁed in terms of the separation factor (˛) : ˛M2+ /Na+ (q/c) = KM2+ /Na+ yNa+ /xNa+ Here, KM2+ /Na+ is the preference factor and is given by the formula KM2+ /Na+ = qM2+ CNa+ 2 CM2+ qNa+ Fig. 6. Langmuir adsorption isotherm for removal of nickel and zinc on Dowex HCR S/S. 3.5.1. Langmuir model The Langmuir isotherm is a commonly applied model for adsorption on a completely homogenous surface with negligible interaction between adsorbed molecules . The model assumes uniform adsorption energies onto the surface and maximum adsorption depends on saturation level of monolayer. Langmuir model can be represented with the following linear equation: Ce 1 Ce = + qe Vm kVm (6) where, q total ion exchange capacity (eq/L); C total ion concentration in solution (eq/L); yNa+ equivalence ratio of Na+ ions in resin xNa+ equivalence ratio of Na+ ions in solution; qM2+ concentration of metal ions in resin (eq/L); CM2+ concentration of metal ions in solution (eq/L); CNa+ concentration Na+ ions in solution (eq/L); qNa+ concentration of Na+ ions in resin (eq/L) In this study separation factors (˛) were calculated as 0.577 and 0.1029 for nickel and zinc removal. According to these values, it was concluded that in removal processes using HCR S/S resins, adsorption tendencies of both ions are satisfying. 3.5. Adsorption isotherms Results obtained for the adsorption of Ni2+ and Zn2+ ions were analyzed with well-known adsorption models such as Langmuir, Freundlich and Temkin. (7) where qe represents the mass of adsorbed heavy metal per unit resin (mg/g), Vm is the monolayer capacity, k is the equilibrium constant and Ce is the equilibrium concentration of the solution (mg/L). k and Vm were determined from the slope, intercept of the Langmuir plot (Fig. 6). 3.5.2. Freundlich model The Freundlich model is known as earliest empirical equation and is shown to be consistent with exponential distribution of active centers, characteristic of heterogeneous surfaces [20,21]. Freundlich equation is: log qe = log Kf + (5) 485 1 log Ce n (8) where Kf and n represent adsorption capacity and intensity, respectively. Kf is an important constant used as relative measure for adsorption efﬁciency. The magnitude of the n shows an indication of the favorability of adsorption. Values of n larger than 1 show the favorable nature of adsorption . The plot of log qe against log Ce , shows data for adsorption of Ni2+ and Zn2+ onto HCR S/S cation exchange resin is ﬁtting well to the Freundlich isotherm (Fig. 7). 3.5.3. Temkin model Temkin adsorption isotherm is expressed as: qe = B ln A + B ln Ce (9) where A is Temkin constant representing adsorbat–adsorbat interactions and B is another constant related with adsorption heat . Temkin isotherm takes into account the adsorbing species– adsorbent interactions. Isotherm constants A and B can be determined from plot of qe versus ln Ce (Fig. 8). From Table 2 it is seen that value of A is larger for Ni 2+ than Zn2+ . This means in cation exchange processes by using HCR S/S, adsorbate/adsorbate interactions are more effective for nickel comparing with zinc. 486 B. Alyüz, S. Veli / Journal of Hazardous Materials 167 (2009) 482–488 Fig. 7. Freundlich adsorption isotherm for removal of nickel and zinc on Dowex HCR S/S. Fig. 9. Kinetics of adsorption of zinc (a) and nickel (b) onto Dowex HCR S/S cation exchange resin. Fig. 8. Temkin adsorption isotherm for removal of nickel and zinc on Dowex HCR S/S. Chemical sorption mechanism for nickel and zinc can be expressed with the following reactions: All constants determined from Langmuir, Freundlich and Temkin isotherms are given in Table 2. 3.6. Kinetics of adsorpiton Ni2+ + 2RNa → R2 Ni + 2Na+ (10) Zn2+ + 2RNa → R2 Zn + 2Na+ (11) Rate constants (k1 and k2 ) of pseudo-ﬁrst- and -second-order kinetics were calculated from experimental data obtained from related reactions. Adsorption kinetics provide valuable information about the mechanism of adsorption . Rate of adsorbate uptake, which is required for selecting optimum operating conditions for the fullscale batch process, can be described with adsorption kinetics . Kinetic studies for nickel and zinc were performed by using different concentrations (50,100,150 mg/L). Optimum conditions were used during these experiments. pH was adjusted to 4 and 6 and resin mass was 0.2 and 0.3 g for nickel and zinc. Samples were taken with different time intervals ranging between 5 and 300 min. Plots of heavy metal concentration against time are in Fig. 9(a) and (b). As seen from Fig. 9(a and b), maximum amount of nickel and zinc ions were adsorbed within the ﬁrst 90 and 120 min, respectively. After these periods adsorption processes exhibit slower rate and reach equilibrium. 3.6.1. Pseudo-ﬁrst-order reaction kinetic Simple linear equation for pseudo-ﬁrst-order reaction kinetic is given below : ln(qe − qt ) = ln qe − k1 t (12) where k1 is the rate constant of the ﬁrst-order adsorption, qt is the amount of heavy metal adsorbed at time ‘t’ (mg/g) and qe is the amount of heavy metal adsorbed at saturation (mg/g). Plot of ln(qe − qt ) versus t allows calculation of the rate constant k1 and qe for nickel and zinc removal (Fig. 10(a) and (b)). Table 2 Isotherm parameters calculated for nickel and zinc removal on Dowex HCR S/S. Metals Ni2+ Zn2+ Langmuir isotherm constants Feundlich isotherm constants Temkin isotherm constants Vm k R2 Kf n R2 A B R2 156.25 222.22 2 4.5 0.93 0.99 68.51 138.48 4.38 1.92 0.89 0.98 337.58 62.82 15.02 37.30 0.80 0.95 B. Alyüz, S. Veli / Journal of Hazardous Materials 167 (2009) 482–488 487 Table 3 Comparison of adsorption rate constants, experimental and calculated qe values for the pseudo-ﬁrst- and -second-order reaction kinetics of removal of nickel and zinc by Dowex HCR S/S. Metals Initial metal concentration (mg/L) qe,experimental (mg/g) Pseudo-ﬁrst-order k1 (1/min) 2+ Ni 50 100 150 Zn2+ 50 100 150 Pseudo-second-order qe,calculated (mg/g) 16.66 32.88 49.56 −2 4.99 × 10 3.90 × 10−2 4.80 × 10−2 8.15 17.63 38.83 24.00 49.56 72.55 2.59 × 10−2 2.51 × 10−2 4.79 × 10−2 13.00 49.21 64.16 R2 qe,calculated (mg/g) R2 0.8843 0.9624 0.9797 −2 3.29 × 10 7.3 × 10−3 3.46 × 10−2 16.80 33.44 50.76 0.9978 0.9996 0.9991 0.9458 0.9596 0.9919 3.56 × 10−2 6.6 × 10−3 2.0 × 10−4 25.18 55.24 74.62 0.9949 0.9783 0.999 k2 (g/mg min) 3.6.2. Pseudo-second-order reaction kinetic Pseudo-second-order reaction kinetic can be expressed as : t 1 t = + qt qe k2 q2e (13) where k2 (g/mg h) is the pseudo-second-order rate constant, qe the amount adsorbed at equilibrium and qt is the amount of metal adsorbed at time ‘t’. Similar to the pseudo-ﬁrst-order reaction kinetic, qe and k2 can be determined from the slope and intercepts of plot t/qt versus t (Fig. 11(a) and (b)). Calculated rate constants (k1 and k2 ), adsorbed amounts of heavy metals per unit resin mass (qe ) and linear regression correlation coefﬁcients (R2 ) for pseudo-ﬁrst- and -second-order reaction kinetics are summarized in Table 3. In pseudo-second-order reaction kinetic, calculated values of qe are closer to experimental values for both nickel and zinc. Furthermore as seen from Table 3, correlation coefﬁcients are higher for second order kinetic studies. Fig. 11. Pseudo-second order reaction kinetics for the adsorption of nickel (a) and zinc (b) onto Dowex HCR S/S cation exchange resin. 4. Conclusions Fig. 10. Pseudo-ﬁrst-order reaction kinetics for the adsorption of nickel (a) and zinc (b) onto Dowex HCR S/S cation exchange resin. The aim of this work was to investigate removal of nickel and zinc from aqueous solutions by using Dowex HCR S/S cation exchange resin. Optimal removal conditions for both metals were determined with batch experiments. Ion exchange process was pH-dependent and optimal removal efﬁciencies for nickel and zinc were obtained at pH 4 and 6, respectively. Adsorption of nickel ions reached equilibrium faster (within 90 min) comparing with zinc ions (within 120 min). Equilibrium distribution coefﬁcients (D) were calculated as 5.80 × 104 and 2.25 × 104 whereas separation factors ˛ were 0.577 and 0.1029 for nickel and zinc removal. Experimental results were evaluated with Langmuir, Freundich and Temkin isotherms. In addition to higher values of correlation coefﬁcients, monolayer capacities (Vm ) determined from Langmuir isotherm and adsorption intensities (n) determined from Freundlich isotherm indicate appropriateness of Langmuir and Freundlich isotherms for both metals. In Temkin isotherm, it was stated 488 B. Alyüz, S. Veli / Journal of Hazardous Materials 167 (2009) 482–488 that adsorbate/adsorbate interactions are weaker for zinc removal due to smaller values of Temkin constant (A). Pseudo-second-order reaction kinetic has provided a realistic description for removal of Ni2+ and Zn2+ with closer experimental and calculated values of qe . Also correlation coefﬁcients are higher in pseudo-second-order kinetics. Experimental and theoretical results of this study demonstrate that Dowex HCR S/S cation exchange resin is suitable for adsorption of nickel and zinc from aqueous solutions. References  F. Gode, E. Pehlivan, A comparative study of two chelating ion exchange resins for the removal of chromium(III) from aqueous solution, J. Hazard. Mater. B100 (2003) 231–243.  S. Veli, B. Alyüz, Adsorption of copper and zinc from aqueous solutions by using natural clay, J. Hazard. Mater. 149 (2007) 226–233.  K.S. Hui, C.Y.H. Chao, S.C. Kot, Removal of mixed heavy metal ions in wastewater by zeolite 4A and residual products from recycled coal ﬂy ash, J. Hazard. Mater. B127 (2005) 89–101.  E. Alvarez-Ayuso, A. Garcia-Sanchez, X. Querol, Puriﬁcation of metal electroplating waste waters using zeolites, Water Res. 37 (2003) 4855–4862.  S.S. Chan, H. Chow, M.H. Wong, Microalge as a bioabsorbents for treating mixture of electroplating and sewage efﬂuent, Biomed. Environ. Sci. 4 (1991) 250–260.  A. Dabrowski, Z. Hubicki, P. Podkoscielny, E. Robens, Selective removal of the heavy metal ions from waters and industrial wastewaters by ion-exchange method, Chemosphere 56 (2004) 91–106.  U. Forstner, G.T.W. Wittman, Metal Pollution in Aquatic Environment, SpringerVerlag, Berlin, 1979.  S. Rengaraj, Y. Kyeong-Ho, M. Seung-Hyeon, Removal of chromium from water and wastewater by ion exchange resins, J. Hazard. Mater. B87 (2001) 273– 287.  D.A. Clifford, Ion exchange and inorganic adsorption, in: Water Quality and Treatment: A Handbook of Community Water Supplies, fourth ed., American Water Works Association, McGraw Hill, New York, 1990.  S.H. Lin, S.L. Lai, H.G. Leu, Removal of heavy metals from aqueous solution by chelating resin in a multistage adsorption process, J. Hazard. Mater. 76 (2000) 139–153.  S. Verbych, N. Hilal, G. Sorokin, M. Leaper, Ion exchange extraction of heavy metal ions from wastewater, Sep. Sci. Technol. 39 (2004) 2031.  K. Halle, K. Fischwasser, B. Fenk, Recovery of metals from electroplating wastes, Technol. Umweltschutz 25 (1982) 120–132.  K. Ohzeki, M. Minorikawa, F. Yokota, I. Nakatsuka, R. Ishida, Enrichment of trace amounts of copper as chelate compounds using a ﬁnely divided ion-exchange resin, Analyst 115 (1990) 23–28.  S. Veli, B. Pekey, Removal of copper from aqueous solutions by ion exchange resins, Fresenius Environ. Bull. 13 (2004) 244–250.  I. Untea, E. Tudorache, C. Florea, Thermodynamic aspects regarding the ion exchange equilibrium in a system Lewatit MP 500A-K2 CrO4 solutions, Rev. Chim. 51 (2000) 123–126.  E. Pehlivan, T. Altun, The study of various parameters affecting the ion exchange of Cu2+ , Zn2+ , Ni2+ , Cd2+ , and Pb2+ from aqueous solution on Dowex 50W synthetic resin, J. Hazard. Mater. B134 (2006) 149–156.  F.E.W. Strelowand, C. Baxter, Separation of tervalent rare earths and scandium from aluminium, iron(III), titanium(IV), and other elements by cation-exchange chromatography in hydrochloric acid-ethanol, Talanta 16 (1969) 1145–1155.  S. Ahmed, S. Chughtai, M.A. Keane, The removal of cadmium and lead from aqueous solution by ion exchange with Na-Y zeolite, Sep. Purif. Technol. 13 (1998) 57–64.  F. Gode, E. Pehlivan, Adsorption of Cr(III) ions by Turkish brown coals, Fuel Process. Technol. 86 (2005) 875–884.  Y.S. Ho, Effect of pH on lead removal from water using tree fern as the sorbent, Bioresour. Technol. 96 (2005) 1292–1296.  E.V. Veliev, T. Öztürk, S. Veli, A.G. Fatullayev, Application of diffussion model for adsorption of azo reactrive dye on pumice, Pol. J. Environ. Stu. 15 (2006) 347–353.  N. Daneshvar, D. Salari, S. Aber, Chromium adsorption and Cr(VI) reduction to trivalent chromium in aqueous solutions by soya cake, J. Hazard. Mater. 94 (2002) 49–61.  I.A.W. Tan, B.H. Hameed, A.L. Ahmad, Equilibrium and kinetic studies on basic dye adsorption by oil palm ﬁbre activated carbon, Chem. Eng. J. 127 (2007) 111–119.  S. Veli, T. Öztürk, Kinetic modelling of adsorption of reactive azo dye on powdered activated carbon and pumice, Fresenius Environ. Bull. 14 (2005) 347–353.  V.K. Gupta, S. Sharma, Removal of zinc from aqueous solutions using bagasse ﬂy ash-a low cost adsorbent, Ind. Eng. Chem. Res. 42 (2003) 6619–6624.  A. Sharma, K.G. Bhattacharyya, Adsorption of chromium(VI) on Azadirachta Indica (Neem) leaf powder, Adsorption 10 (2004) 327–338.  Y.S. Ho, G. McKay, Sorption of dye from aqueous solution by peat, J. Chem. Eng. 70 (1998) 115–124.